#------------------------------------------------------------------------------
#$Date: 2016-02-20 00:18:51 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176760 $
#$URL: svn://www.crystallography.net/cod/cif/2/01/87/2018786.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2018786
loop_
_publ_author_name
'Bond, Andrew D.'
'Warner, Terence E.'
_publ_section_title
;
 Copper scandium zirconium phosphate: occupancy of the M1 and
 M2 sites in the temperature range 100--300K
;
_journal_coeditor_code           KU3084
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              105
_journal_page_last               110
_journal_paper_doi               10.1107/S0108270113000553
_journal_volume                  69
_journal_year                    2013
_chemical_formula_iupac          'Cu1.92 O12 P3 Sc Zr'
_chemical_formula_moiety         'Cu1.92 O12 P3 Sc Zr'
_chemical_formula_sum            'Cu1.92 O12 P3 Sc Zr'
_chemical_formula_weight         543.09
_chemical_name_systematic
;
Copper scandium zirconium phosphate
;
_space_group_IT_number           167
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   8.9344(5)
_cell_length_b                   8.9344(5)
_cell_length_c                   22.0918(16)
_cell_measurement_reflns_used    2369
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      28.07
_cell_measurement_theta_min      3.21
_cell_volume                     1527.19(16)
_computing_cell_refinement       'SAINT (Bruker, 2010)'
_computing_data_collection       'APEX2 (Bruker, 2010)'
_computing_data_reduction        'SAINT and XPREP (Bruker, 2010)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 2008)'
_computing_publication_material  'SHELXTL (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXTL (Sheldrick, 2008)'
_computing_structure_solution    'SHELXTL (Sheldrick, 2008)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker Nonius X8 APEXII CCD area-detector'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0432
_diffrn_reflns_av_sigmaI/netI    0.0183
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            15401
_diffrn_reflns_theta_full        28.23
_diffrn_reflns_theta_max         28.23
_diffrn_reflns_theta_min         4.53
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    6.127
_exptl_absorpt_correction_T_max  0.787
_exptl_absorpt_correction_T_min  0.545
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2010)'
_exptl_crystal_colour            beige
_exptl_crystal_density_diffrn    3.543
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1546
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.04
_refine_diff_density_max         0.486
_refine_diff_density_min         -0.514
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.194
_refine_ls_matrix_type           full
_refine_ls_number_parameters     58
_refine_ls_number_reflns         422
_refine_ls_number_restraints     18
_refine_ls_restrained_S_all      1.173
_refine_ls_R_factor_all          0.0291
_refine_ls_R_factor_gt           0.0265
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0042P)²+15.7557P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0561
_refine_ls_wR_factor_ref         0.0570
_reflns_number_gt                387
_reflns_number_total             422
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            ku3084.cif
_cod_data_source_block           I_200K
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_database_code               2018786
_cod_database_fobs_code          2018786
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+5/6'
'x-y+2/3, -y+1/3, -z+5/6'
'-x+2/3, -x+y+1/3, -z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+7/6'
'x-y+1/3, -y+2/3, -z+7/6'
'-x+1/3, -x+y+2/3, -z+7/6'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z-1/6'
'-x+y+2/3, y+1/3, z-1/6'
'x+2/3, x-y+1/3, z-1/6'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+1/6'
'-x+y+1/3, y+2/3, z+1/6'
'x+1/3, x-y+2/3, z+1/6'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_symmetry_multiplicity
Cu Cu1 0.1660(6) 0.570(2) 0.1679(3) 0.023(3) Uani d PU 0.210(13) 1
Cu Cu2 0.1070(11) 0.4216(11) 0.1311(3) 0.017(3) Uani d PU 0.064(3) 1
Cu Cu3 0.179(3) 0.639(7) 0.1768(13) 0.014(8) Uani d PU 0.044(13) 1
Zr Zr1 0.0000 0.0000 0.14248(3) 0.00594(18) Uani d SP 0.50 3
Sc Sc1 0.0000 0.0000 0.14248(3) 0.00594(18) Uani d SP 0.50 3
P P1 0.0000 0.28708(12) 0.2500 0.0072(3) Uani d S 1 2
O O1 0.0064(4) 0.1945(4) 0.19295(11) 0.0184(6) Uani d . 1 1
O O2 0.1615(3) 0.4697(3) 0.24963(13) 0.0148(5) Uani d . 1 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Zr Zr -2.9673 0.5597 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sc Sc 0.2519 0.3716 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O2 Cu1 O2 . 26_455 171.9(5)
O2 Cu1 O1 . 26_455 110.5(2)
O2 Cu1 O1 26_455 26_455 63.09(16)
O2 Cu1 O2 . 3_565 72.3(4)
O2 Cu1 O2 26_455 3_565 113.6(6)
O1 Cu1 O2 26_455 3_565 106.6(5)
O2 Cu1 O2 . 27 111.5(6)
O2 Cu1 O2 26_455 27 70.3(3)
O1 Cu1 O2 26_455 27 121.0(4)
O2 Cu1 O2 3_565 27 124.5(2)
O2 Cu1 O1 . . 55.8(3)
O2 Cu1 O1 26_455 . 117.7(6)
O1 Cu1 O1 26_455 . 89.1(3)
O2 Cu1 O1 3_565 . 127.93(15)
O2 Cu1 O1 27 . 82.0(5)
O2 Cu1 O2 . 6 50.46(14)
O2 Cu1 O2 26_455 6 122.0(2)
O1 Cu1 O2 26_455 6 61.33(11)
O2 Cu1 O2 3_565 6 96.7(3)
O2 Cu1 O2 27 6 129.5(6)
O1 Cu1 O2 . 6 47.93(14)
O2 Cu2 O1 26_455 . 162.1(4)
O2 Cu2 O2 26_455 27 81.9(3)
O1 Cu2 O2 . 27 116.0(4)
O2 Cu2 O2 26_455 . 114.0(4)
O1 Cu2 O2 . . 60.07(19)
O2 Cu2 O2 27 . 109.5(4)
O2 Cu2 O1 26_455 26_455 59.2(2)
O1 Cu2 O1 . 26_455 103.0(3)
O2 Cu2 O1 27 26_455 141.0(3)
O2 Cu2 O1 . 26_455 89.1(2)
O2 Cu2 O2 26_455 30_455 120.6(3)
O1 Cu2 O2 . 30_455 58.7(2)
O2 Cu2 O2 27 30_455 105.5(3)
O2 Cu2 O2 . 30_455 117.8(2)
O1 Cu2 O2 26_455 30_455 94.3(3)
O2 Cu2 O2 28 30_455 54.29(17)
O2 Cu2 O2 26_455 6 113.9(3)
O1 Cu2 O2 . 6 48.89(16)
O2 Cu2 O2 27 6 155.1(4)
O2 Cu2 O2 . 6 47.30(14)
O1 Cu2 O2 26_455 6 58.38(16)
O2 Cu2 O2 28 6 118.8(2)
O2 Cu2 O2 30_455 6 83.57(18)
O2 Cu3 O2 26_455 . 142(3)
O2 Cu3 O2 26_455 3_565 136(3)
O2 Cu3 O2 . 3_565 81.4(10)
O2 Cu3 O1 26_455 26_455 62.2(7)
O2 Cu3 O1 . 26_455 105.3(14)
O2 Cu3 O1 3_565 26_455 124.1(17)
O2 Cu3 O1 26_455 3_565 90.7(16)
O2 Cu3 O1 . 3_565 125.1(16)
O2 Cu3 O1 3_565 3_565 51.3(12)
O1 Cu3 O1 26_455 3_565 85.0(11)
O1 Zr1 O1 . 3 93.01(10)
O1 Zr1 O1 . 2 93.01(10)
O1 Zr1 O1 3 2 93.01(10)
O1 Zr1 O2 . 29_445 173.29(11)
O1 Zr1 O2 3 29_445 93.59(11)
O1 Zr1 O2 2 29_445 87.82(11)
O1 Zr1 O2 . 28 93.59(11)
O1 Zr1 O2 3 28 87.82(11)
O1 Zr1 O2 2 28 173.29(11)
O2 Zr1 O2 29_445 28 85.48(11)
O1 Zr1 O2 . 30_455 87.82(10)
O1 Zr1 O2 3 30_455 173.29(11)
O1 Zr1 O2 2 30_455 93.59(11)
O2 Zr1 O2 29_445 30_455 85.48(11)
O2 Zr1 O2 28 30_455 85.48(11)
O1 P1 O1 . 6 111.7(2)
O1 P1 O2 . . 107.46(16)
O1 P1 O2 6 . 111.16(15)
O1 P1 O2 . 6 111.16(15)
O1 P1 O2 6 6 107.46(16)
O2 P1 O2 . 6 107.8(2)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Cu1 O2 . 2.005(5)
Cu1 O2 26_455 2.028(5)
Cu1 O1 26_455 2.607(6)
Cu1 O2 3_565 2.756(16)
Cu1 O2 27 2.830(13)
Cu1 O1 . 2.965(15)
Cu1 O2 6 3.240(5)
Cu2 O2 26_455 2.124(8)
Cu2 O1 . 2.229(7)
Cu2 O2 27 2.258(8)
Cu2 O2 . 2.660(8)
Cu2 O1 26_455 2.761(9)
Cu2 O2 28 2.923(9)
Cu2 O2 30_455 3.325(9)
Cu2 O2 6 3.361(8)
Cu3 O2 26_455 2.09(3)
Cu3 O2 . 2.16(4)
Cu3 O2 3_565 2.25(5)
Cu3 O1 26_455 2.62(2)
Cu3 O1 3_565 3.15(6)
Zr1 O1 . 2.042(2)
Zr1 O1 3 2.042(2)
Zr1 O1 2 2.042(2)
Zr1 O2 29_445 2.117(2)
Zr1 O2 28 2.117(2)
Zr1 O2 30_455 2.117(2)
P1 O1 . 1.524(2)
P1 O1 6 1.524(2)
P1 O2 . 1.546(2)
P1 O2 6 1.546(2)
